Synthesis of Nickel-Encapsulated Carbon Nanocapsules and Cup-Stacked-Type Carbon Nanotubes via Nickel-Doped Fullerene

Nickel(Ni) doped C60 nanowhiskers (NWs) were synthesized by a liquid-liquid interfacial precipitation method using a C60saturated toluene solution and isopropanol with Ni nitrate hexahydrate Ni(NO3)2·6H2O. By varying the heating temperature of Ni-doped C60 NWs, two types of one-dimensional carbon nanostructures were produced. By heating the NWs at 973 and 1173 K, carbon nanocapsules (CNCs) that encapsulated Ni nanoparticles were produced. The Ni-encapsulated CNCs joined one dimensionally to form chain structures. Upon heating the NWs to 1373 K, cup-stacked-type carbon nanotubes were synthesized.


Method
C 60 powders were dissolved in toluene to prepare a C 60saturated solution with a solubility of 2.8 g/L.Ni nitrate hexahydrate [Ni(NO 3 ) 2 •6H 2 O] was dissolved in 2-propanol with concentrations of 0.01 M and 0.68 M (hereafter labeled as specimens A and B, resp.).The C 60 toluene solution was poured into a glass vial, and the 2-propanol was then added to form a liquid-liquid interface.After the vial was maintained at 278 K for one week, the solution was filtered to extract precipitates.The precipitates were dried and heated in high vacuum at 973, 1173, and 1323 K for 1 h.Next, the specimens were dispersed on microgrids and observed by transmission electron microscopy (TEM).Thermogravimetric analyses (TGA) and differential thermal analyses (DTA) of the specimens were performed in a nitrogen flow.Figure 3 shows TGA and DTA curves of the Ni-doped NWs in specimen A and C 60 bulk crystals.For C 60 bulk crystals, the DTA curve starts to decrease around 773 K. On the other hand, no change is observed in the TGA curve around this temperature.This shows that the mass of the specimen remained unchanged, whereas the structure changed.The transformation from a crystalline to an amorphous configuration of C 60 molecules starts at this temperature [27].Around 1173 K, the TGA curve decreases, and a downward peak is observed in the DTA curve, which shows that an endothermic reaction occurred.Furthermore, it has been reported that sublimation of C 60 molecules takes place at this temperature [27].On the other hand, for the Ni-doped NWs, an upward peak was observed in the DTA curve around 773 K, which corresponds to an exothermic reaction.No change is observed in the TGA curve around this temperature.TEM observations showed that grain coarsening of Ni particles started near this temperature.This TEM result suggests that the upward peak around 773 K was caused by the grain coarsening of Ni particles.

Results and Discussion
Around 1123 K, the TGA curve decreases and the DTA curve shows a downward peak.This implies that the sublimation of C 60 molecules occurred, as similarly observed in C 60 bulk crystals.Note that the sublimation temperature of C 60 molecules in the Ni-doped NWs is approximately 50 K lower than that in the C 60 bulk crystals.From this result, we infer that Ni particles act as catalysts for the weakening of intermolecular C 60 molecular bonds.
On the basis of the results of TGA and DTA, we heated the specimens to temperatures higher than 973 K and observed them by TEM.Figures 4(a    of CNTs, and the graphene layers were aligned parallel to the surfaces of Ni particles.Thus, CNTs were produced by the continuous precipitation of graphene cones and the continuous movement of Ni particles.However, for CNC formation, the movement of Ni particles and the precipitation of graphene shells are intermittent. In this experiment, cup-stacked-type CNTs were produced at the highest temperature (1373 K).As observed in Figures 4(b) and 5(a), the Ni particles in the specimens heated at temperatures lower than 1173 K formed spherical shapes, whereas Ni particles in the specimens heated to 1373 K formed clear crystal habits.At higher temperatures, the metal particles show more stable shapes surrounded by crystal planes with lower surface energies.Cup-stacked-type CNTs are formed by one-directional continuous precipitation of graphitic cones from metal particles having such clear crystal habits [30][31][32][33][34][35][36][37][38][39].The solubility limit of carbon atoms in metals also increases at higher temperatures, and the precipitation speed increases.We infer that both the formation of crystal habits and the increase in precipitation speed promote the production of cup-stacked-type CNTs.

Conclusion
Ni-doped C 60 NWs synthesized by the liquid-liquid interfacial precipitation method allow us to produce Ni-encapsulated CNCs and cup-stacked-type CNTs.In particular, the CNCs form chain structures.The two types of one-dimensional carbon nanostructures were produced using Ni-doped C 60 NWs by varying heating temperature.
Other transition metals such as iron and cobalt can be doped into fullerene NWs using similar synthetic methods, and CNCs encapsulating nanoparticles of various metal elements can be produced using NWs.

Figure 1 (
Figure 1(a) shows a bright-field image of an as-precipitated Ni-doped C 60 NW in specimen A. The diameter of this NW is 740 nm.The surfaces of the Ni-doped NWs were porous, as shown in Figure 1(b).Figure 2(a) shows a brightfield image of an as-precipitated Ni-doped C 60 NW in specimen B. The diameter of this NW is 240 nm.The NWs showed undulating surfaces.Ni particles with a face-centered

Figure 1 :
Figure 1(a) shows a bright-field image of an as-precipitated Ni-doped C 60 NW in specimen A. The diameter of this NW is 740 nm.The surfaces of the Ni-doped NWs were porous, as shown in Figure 1(b).Figure 2(a) shows a brightfield image of an as-precipitated Ni-doped C 60 NW in specimen B. The diameter of this NW is 240 nm.The NWs showed undulating surfaces.Ni particles with a face-centered

Figure 2 :Figure 3 :Figure 4 :
Figure 2: (a) Bright-field images of Ni-doped C 60 nanowhiskers synthesized using isopropyl alcohol with concentration of 0.68 M Ni(NO 3 ) 2 •6H 2 O.The arrows indicate Ni particles in dents.(b) High-resolution image of Ni particles in the NW in (a).

Figure 5 :
Figure 5: (a) Bright-field images of Ni-encapsulated carbon nanocapsules prepared by heating Ni-doped C 60 nanowhiskers (specimen B) at 1173 K.The nanocapsules form chain structures.(b) High-resolution image of the chain of Ni-encapsulated carbon nanocapsules.
) and 4(b) show bright-field and high-resolution images of specimen A after heating at 973 K, respectively.Ni-encapsulated CNCs are formed by this heat treatment.The diameter of the CNCs ranged from 12 to 51 nm.The diameter of the encapsulated Ni particles ranged from 8 to 33 nm.A portion of the CNCs aligned one dimensionally to form chain structures, as shown in Figure 4(c).Such chain structures have also been produced by arc discharge [28, 29].As shown in Figure 4(b), Ni particles were attached on the tips of the chains, indicating that the chain structures were produced by the cycles of the precipitation of graphene shells around Ni particles and the movement of the Ni particles.Note that in Figure 4(b), the Ni particle protrudes from the center of the hollow region of the CNC.This state corresponds to the movement of the Ni particle from the precipitated graphene shell.Figures 5(a) and 5(b) show bright-field and high-resolution images of specimen B after heating it at 1173 K. Niencapsulated CNCs and their chain structures were formed.The formation rate of CNC chains in this specimen was higher than that in specimen A owing to a higher concentration of Ni particles.By heating Ni-doped C 60 NWs in specimen B to 1323 K, cup-stacked-type carbon nanotubes (CNTs) were produced, as shown in Figure6.Ni particles were attached to the tip

Figure 6 :
Figure 6: (a) Cup-stacked-type carbon nanotube synthesized by heating Ni-doped C 60 nanowhiskers (specimen B) at 1323 K. (b) High-resolution image of the cup-stacked-type carbon nanotube depicted in (a).